The marginal fit of selective laser meltingefabricated metal crowns: An in vitro study Dan Xu, MS,a Nan Xiang, MS,b and Bin Wei, DDS, MS, PhDc Stomatology Special Consultation Clinic, Ninth People’s Hospital, Shanghai Jiao Tong University School of Medicine, Shanghai, PR China Statement of problem. The selective laser melting technique is attracting interest in prosthetic dentistry. The marginal ﬁt is a key criterion for ﬁxed restorations. Purpose. The purpose of the study was to evaluate the marginal ﬁt of cast cobalt-chromium alloy crowns versus the ﬁt of selective laser meltingefabricated crowns. Material and methods. The marginal gap widths of 36 single crowns (18 selective laser meltingefabricated cobalt-chromium metal crowns and 18 cobalt-chromium cast crowns) were determined with a silicone replica technique. Each crown specimen was cut into 4 sections, and the marginal gap width of each cross section was evaluated by stereomicroscopy (100). The Student t test was used to evaluate whether signiﬁcant differences occurred in the marginal gap widths between the selective laser meltingefabricated and cast cobalt-chromium metal crowns (a¼.05). Results. The mean marginal gap width of the cast crowns (170.19 mm) was signiﬁcantly wider than that of the selective laser meltingefabricated crowns (102.86 mm). Conclusions. Selective laser meltingefabricate cobalt-chromium dental crowns found improved marginal gap widths compared with traditional cast crowns. (J Prosthet Dent 2014;112:1437-1440)
Clinical Implications In the present in vitro study, selective laser meltingefabricated cobalt-chromium dental crowns exhibited signiﬁcantly improved marginal gap widths compared with traditional cast crowns. This ﬁnding may indicate that selective laser melting crowns are more acceptable. Selective laser melting (SLM) is a rapid prototyping method for fabricating metal products directly from computer-aided design (CAD) data. Automated fabrication is accomplished layer-by-layer by selectively fusing together metal powders.1-3 Compared with the traditional casting method, SLM offers several advantages, such as a higher deﬁnitive product density, reduced manufacturing time and costs, minimization of human errors, and the prevention of casting defects.4-7 The
SLM technique is attracting interest in prosthetic dentistry. Because SLM is a relatively new manufacturing technique, it requires extensive evaluation before it can be used to produce prostheses for clinical use. An important consideration is the marginal ﬁt, which is a key criterion for ﬁxed restorations. Once the restoration is placed onto the tooth, the gap between the gingival margin and the tooth preparation serves as a connection to the oral environment. Several clinical
trials have emphasized the importance of marginal ﬁt for the clinical success of ﬁxed restorations.8-12 If the crown and the abutment do not ﬁt well, then problems, such as gingival bleeding or alveolar bone reaction, may occur. It is not clinically desirable that a crown should have a perfect ﬁt with no marginal gap13 because there must be space for the luting agent. Clinical evaluation procedures should be comfortable and convenient both to the patient and the dentist. However, if the
Supported by Shanghai Leading Academic Discipline Project (Project Number: T0202, S30206) and the Science and Technology Committee of Shanghai (08DZ2271100, 12441903001, and 13140902701). a
Postgraduate student, Department of Prosthodontics. Postgraduate student, Department of Prosthodontics. c Associate Professor, Department of Prosthodontics, Stomatology Special Consltation Clinic. b
Xu et al
Volume 112 Issue 6
2 Metal crown coping seated on original master die after application.
1 Standardized stainless-steel die.
marginal discrepancies are too large, then the luting agent will be exposed to the oral environment. Thus, the larger the marginal discrepancy is, the faster the rate of cement dissolution will be.13 Subsequent failure of the cement seal and bacterial percolation can cause pulpal inﬂammation and even pulpal necrosis.14 Many studies have compared the marginal ﬁt of complete metal, metal ceramic, and/or ceramic crowns that were fabricated either through CAD/ computer-aided manufacturing systems or traditional casting machines.15-19 Studies performed with various materials and techniques reported a wide range of marginal gaps, which ranged from 10 to 500 mm, mean (SD) range, 10 50 mm to 500 100 mm.10,20 In a study of single cast crowns, 50% of the marginal gap values exceeded 150 mm.20 In another report, single metal alloy crowns fabricated by computer-supported laser-melting technology had mean marginal gap widths of 74 to 99 mm.21 Comparing these studies is difﬁcult because they differ markedly in many aspects of the fabrication process, including impression making, deﬁnitive casts, casting, and scanning. Moreover, such differences cannot be avoided because cast crowns are fabricated with an entirely manual procedure. In contrast, human errors can be minimized by fabricating crowns with SLM. A literature review revealed no prior investigation of the
marginal ﬁt of SLM-fabricated cobaltchromium (CoCr) metal crowns. Therefore, in the present study, the marginal ﬁts of SLM-fabricated and conventional cast CoCr metal crowns were compared. The null hypothesis was that the average marginal gap widths would not be signiﬁcantly different between the SLM-fabricated and cast single crowns.
MATERIAL AND METHODS Thirty-six single crowns were examined in this study (18 SLM-fabricated CoCr metal crowns and 18 CoCr cast crowns). To fabricate the metal crowns, a maxillary premolar crown preparation was simulated by using a stainless-steel die with a height of 6.0 mm (with assuming a 2-mm ﬂat occlusal reduction), a uniform heavy chamfer ﬁnish line of 1.0 mm in width, and a total occlusal convergence of 5 degrees (Fig. 1). The die was manually prepared by using tungsten carbide burs (MANI Inc) and trimmed on a survey plate (Combilabor CL-MF 2000; Heraeus). The specimens were prepared from a CoCr alloy (Wirbond Cþ; Bego Dental) in casting and powder form. The die was scanned with a dental system scanner (D700; 3Shape), and a 3-dimensional computer cast was created. SLM restorations were fabricated with an SLM system (Bego Medifacturing System; Bego Medical) based on the 3-dimensional computer cast.
The Journal of Prosthetic Dentistry
SLM specimens were fabricated layerby-layer with a machine that was equipped with an ytterbium ﬁber laser. The laser produced a beam with a wavelength range of 1060 to 1100 nm, and a maximum power of 200 W. The laser speed was less than 7000 mm/s, and the laser-beam diameter was approximately 0.1 mm. Wax patterns for investment casting were prepared. The crowns were cast in a standard broken-arm centrifugal casting machine (T.I.M. 500 plus; Dentalfarm), in accordance with the manufacturer’s instructions. Brieﬂy, the wax pattern was made on a gypsum die duplicated from the metal die by using a polyvinyl siloxane impression material (Empress II; 3M ESPE) and invested in a casting investment material (Whip Mix Corp). During heating, the wax was eliminated while the casting investment materials solidiﬁed. The originally waxﬁlled cavity was ﬁlled with the heated metal solution. The metal solution solidiﬁed, and a metal crown was formed. To determine the marginal ﬁt, each crown was ﬁlled with light-body polyvinyl siloxane impression material (Empress II; 3M ESPE), placed onto the abutment tooth of the master cast, and loaded with a torque of 50 N in the apical direction (Fig. 2). The thin polyvinyl siloxane layer represented the gap width between the inner surface of the crown (including the crown margin) and the surface of the die. After the light-body impression material had set, the crown was removed from the
Xu et al
3 Silicone replica with mesiodistal and buccolingual sectioning directions. master cast, with the thin impression material layer remaining on the crown. The ﬁlm was stabilized with a contrasting heavy-body polyvinyl siloxane. Materials were used in accordance with manufacturers’ instructions. The premolar replica was sectioned into 4 parts by 2 cuts each in the mesiodistal and buccolingual directions (Fig. 3). Measurements in each of these 2 directions were made for every part, which totaled 8 measurements. The thickness of the light-body polyvinyl siloxane was measured with a microscope (Stemi 2000C; Carl Zeiss) at 100 magniﬁcation. Cross sections were adjusted horizontally on the modeling clay, with the microscope plate maintained at a parallel orientation to achieve a vertical observation angle. The distance (in mm) was determined with a digital measuring device (SPOT version 4.6; Carl Zeiss), which was calibrated at regular intervals. At each cross section, the marginal gap was measured. The width was measured as the perpendicular distance from the internal surface at the margin of the restoration to the preparation12 (Fig. 4). The marginal ﬁt of each crown was determined as the average of all 8 measurements. The experimental results were subjected to statistical analysis with software (SAS 8.0; SAS Institute). The normality of the marginal gap data distribution of each group was tested, and the results indicated homogeneity of variance (P>.05). The Student t test
Xu et al
4 Photograph, showing marginal gap (100).
was used to assess the signiﬁcance of differences in the performances of the 2 materials (a¼.05).
RESULTS The mean (standard deviation) of the marginal gap width for the SLMfabricated crown group was 102.86 40.54 mm (95% conﬁdence interval [CI], 54.55-185.94 mm). The corresponding values for the cast crown group were 170.19 66.17 mm (95% CI, 96.17-337.63 mm). The marginal gap widths differed signiﬁcantly between the 2 groups (P>.05 by the AndersoneDarling test; P